General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.8 g/cm³ Show Material materials with Density of 7.8 g/cm³ |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 217 GPa Show Material materials with Elastic modulus of 217 GPa |

20.0 °C | 212 GPa Show Material materials with Elastic modulus of 212 GPa | |

100.0 °C | 207 GPa Show Material materials with Elastic modulus of 207 GPa | |

200.0 °C | 199 GPa Show Material materials with Elastic modulus of 199 GPa | |

300.0 °C | 192 GPa Show Material materials with Elastic modulus of 192 GPa | |

400.0 °C | 184 GPa Show Material materials with Elastic modulus of 184 GPa | |

500.0 °C | 175 GPa Show Material materials with Elastic modulus of 175 GPa | |

600.0 °C | 164 GPa Show Material materials with Elastic modulus of 164 GPa | |

Poisson's ratio | 20.0 °C | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] |

Reduction of area | 20.0 °C | 58 % Show Material materials with Reduction of area of 58 % |

Tensile strength | 20.0 °C | 620 MPa Show Material materials with Tensile strength of 620 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K | |

20.0 °C | 1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K | ||

100.0 °C | 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.25E-5 1/K | ||

200.0 °C | 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.3E-5 1/K | ||

300.0 °C | 1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K | ||

400.0 °C | 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.41E-5 1/K | ||

500.0 °C | 1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K | ||

600.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | ||

Unlock all property charts | |||

Melting point | 1382 - 1529 °C Show Material materials with Melting point of 1382 - 1529 °C | Typical for Chromium Steel | |

Specific heat capacity | -100.0 °C | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) | |

20.0 °C | 461 J/(kg·K) Show Material materials with Specific heat capacity of 461 J/(kg·K) | ||

100.0 °C | 479 J/(kg·K) Show Material materials with Specific heat capacity of 479 J/(kg·K) | ||

200.0 °C | 499 J/(kg·K) Show Material materials with Specific heat capacity of 499 J/(kg·K) | ||

300.0 °C | 517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) | ||

400.0 °C | 536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) | ||

500.0 °C | 558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) | ||

600.0 °C | 587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 44.9 W/(m·K) Show Material materials with Thermal conductivity of 44.9 W/(m·K) | |

100.0 °C | 46.2 W/(m·K) Show Material materials with Thermal conductivity of 46.2 W/(m·K) | ||

200.0 °C | 45.5 W/(m·K) Show Material materials with Thermal conductivity of 45.5 W/(m·K) | ||

300.0 °C | 43.1 W/(m·K) Show Material materials with Thermal conductivity of 43.1 W/(m·K) | ||

400.0 °C | 40.4 W/(m·K) Show Material materials with Thermal conductivity of 40.4 W/(m·K) | ||

500.0 °C | 37.7 W/(m·K) Show Material materials with Thermal conductivity of 37.7 W/(m·K) | ||

600.0 °C | 34.9 W/(m·K) Show Material materials with Thermal conductivity of 34.9 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 12.5 mm²/s Show Material materials with Thermal diffusivity of 12.5 mm²/s | |

100.0 °C | 12 mm²/s Show Material materials with Thermal diffusivity of 12 mm²/s | ||

200.0 °C | 11 mm²/s Show Material materials with Thermal diffusivity of 11 mm²/s | ||

300.0 °C | 9.8 mm²/s Show Material materials with Thermal diffusivity of 9.8 mm²/s | ||

400.0 °C | 8.6 mm²/s Show Material materials with Thermal diffusivity of 8.6 mm²/s | ||

500.0 °C | 7.3 mm²/s Show Material materials with Thermal diffusivity of 7.3 mm²/s | ||

600.0 °C | 5.9 mm²/s Show Material materials with Thermal diffusivity of 5.9 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 2.32E-7 Ω·m Show Material materials with Electrical resistivity of 2.32E-7 Ω·m |

100.0 °C | 2.77E-7 Ω·m Show Material materials with Electrical resistivity of 2.77E-7 Ω·m | |

200.0 °C | 3.47E-7 Ω·m Show Material materials with Electrical resistivity of 3.47E-7 Ω·m | |

300.0 °C | 4.35E-7 Ω·m Show Material materials with Electrical resistivity of 4.35E-7 Ω·m | |

400.0 °C | 5.38E-7 Ω·m Show Material materials with Electrical resistivity of 5.38E-7 Ω·m | |

500.0 °C | 6.56E-7 Ω·m Show Material materials with Electrical resistivity of 6.56E-7 Ω·m | |

600.0 °C | 7.95E-7 Ω·m Show Material materials with Electrical resistivity of 7.95E-7 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.42 - 0.5 % Show Material materials with Carbon of 0.42 - 0.5 % |

Chromium | 0.4 - 0.6 % Show Material materials with Chromium of 0.4 - 0.6 % |

Manganese | 0.5 - 0.8 % Show Material materials with Manganese of 0.5 - 0.8 % |

Phosphorus | 0.04 % Show Material materials with Phosphorus of 0.04 % |

Silicon | 0.4 % Show Material materials with Silicon of 0.4 % |

Sulfur | 0.035 % Show Material materials with Sulfur of 0.035 % |